J Dent Shiraz Univ Med Sci., Dec. 2013; 14(4): 178-183.
Safari A., et al. Original Article
Effect of Beverages on the Hardness and Tensile Bond Strength of Temporary Acrylic Soft Liners to Acrylic Resin Denture Base Safari A.a, Vojdani M.b, Mogharrabi S.c, Iraji Nasrabadi N.d, Derafshi R.a a
Dept. of Prosthodontics, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran Dental Biomaterial Research Center, Dept. of Prosthodontics, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran c Assistant professor, Dept. of Prosthodontics, School of Dentistry, Jondi Shapour University of Medical Sciences, Ahvaz, Iran d Dentist, Member of Student Research Committee, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran b
KEY WORDS Beverage; Hardness; Tensile Bond Strength; Soft Liner
Received April 2013; Received in revised form May 2013; Accepted June 2013.
ABSTRACT Statement of Problem: Two potential problems commonly identified with a denture base incorporating a resilient liner are failure of the bond between acrylic resin and soft liner material, and loss of resiliency of the soft liner over time. Since patients may drink different beverages, it is important to evaluate their effects on physical properties of soft lining materials. Purpose: The objective of this in vitro study was to evaluate the effect of different beverages on the hardness of two temporary acrylic-based soft lining materials and their bond strength to the denture base resin. Materials and Method: For the hardness test; a total of 80 rectangular specimens (40mm×10mm×3mm) were fabricated from a heat-polymerized polymethylmethacrylate. Two commercially auto-polymerized acrylic resin-based resilient liners; Coe-Soft and Visco-gel were prepared according to the manufacturers’ instructions and applied on the specimens. For the tensile test, 160 cylindrical specimens (30mm×10mm) were prepared. The liners were added between specimens with a thickness of 3 mm. The specimens of both soft liners were divided into 4 groups (n=10) and immersed in distilled water as the control group, Coca-Cola, 8% and 50% ethanol. All groups were stored in separate containers at 37oC for 12 days. All beverages were changed daily. The hardness was determined using a Shore A durometer and tensile bond strength was determined in a ZwickRoell testing machine at a cross-head speed of 5mm/min. The results were analyzed using two-way ANOVA. Results: There was no significant interaction between the soft liners and the drinks for both hardness (p= 0.748) and bond strength (p= 0.902). There were statistically significant differences between all drinks for both hardness (p< 0.001) and bond strength (p< 0.05). Conclusion: Within the limitations of this study, it seems that drinking Coca-Cola and alcoholic beverages would not be potentially causing any problems for the temporary acrylic soft liners.
Corresponding Author: Iraji Nasrabadi N., Dentist, Member of Student Research Committee, School of Dentistry, Shiraz University of Medical Sciences, Shiraz, Iran Tel: +98-9177122230 Email: [email protected]
Cite this article as: Safari A., Vojdani M., Mogharrabi S., Iraji Nasrabadi N., Derafshi R. Effect of Beverages on the Hardness and Tensile Bond Strength of Temporary Acrylic Soft Liners to Acrylic Resin Denture Base. J Dent Shiraz Univ Med Sci., Dec. 2013; 14(4): 178-183.
Introduction Resilient soft lining materials can be helpful for the management of patients with removable prosthesis who are
unable to bear the hard denture base due to thin underlying mucosa, resorption of the residual ridge, severe undercuts and heavy and unequal distribution of occlusal 178
Effect of Beverages on the Hardness and Tensile Bond Strength of Temporary Acrylic Soft Liners to Acrylic …
Safari A., et al.
Table 1 List of materials used in this study Product
Type of polymerization
Meilodent Heat-polymerized denture base polymer Coe-Soft Auto-polymerized acrylic resin-based resilient liner Visco-gel Auto-polymerized acrylic resin-based resilient liner
loads [1-5]. Short-term-use soft liners can be employed as tissue conditioners, functional impression materials and temporary reliners of ill-fitting removable dentures [6-7]. These materials can also be used as the interim liners in the healing periods after implant placement . Soft liners can be either heat-polymerized or autopolymerized [3, 9] and they are usually provided as powder and liquid. The powder consists of polyethylmethacrylate (PEMA) and the liquid contains ethyl alcohol (as solvent) and an aromatic ester (di-butyl phthalate) as the plasticizer agent which is responsible for maintaining material softness [8, 10]. The efficiency of these materials is based on their cushioning effect and they lose their resiliency and become harder after clinical use. The temporary nature of these types of materials is because, in their clinical use, the alcohol and the plasticizer leach out from their structure and water or saliva is absorbed by them which eventually lead to the loss of viscoelasticity and their compliance [11-13]. Softness is a desirable property of resilient liners. Their optimum thickness has been reported to be approximately 2.5 to 3 mm to provide good shock absorption [14-15]. Another serious problem with these materials is bond the failure between the soft liner and the denture base. Any other desirable properties of a denture liner would not be beneficial, unless a good bond to the denture base is achieved. Other problems with soft liners include contamination and accumulation of microorganisms, plaque and calculus formation, poor tear and tensile strength [3, 8, 14-16]. Several studies have been carried out about the effects of water and denture cleansers on the properties of soft lining materials [7, 9, 17-18]. But there are few published articles in regard to the effect of beverages on the hardness and bond strength of resilient soft liner materials. Therefore, the aim of this study was to evaluate the effect of different beverages on the hardness and tensile bond strength of 2 acrylic auto-polymerizing temporary soft liners.
Powder/ Manufacturer Liquid Ratio 23.4g : 10ml Heraeus Kulzer, Hanau, Germany 11g : 8ml GC America Inc., Alsip, Ill 3g : 2.2ml Dentsply, De Trey GmbH, Konstanz, Germany
The null hypothesis is that the hardness values of the soft liners stored in beverages are the same as those of specimens immersed in distilled water and increasing the hardness does not change the bond strength. Materials and Method In this in vitro experimental study, two commercially available acrylic resin-based temporary soft liners were chosen for evaluation. The brand of the resilient liners and the denture base resin material, their manufacturers, powder/liquid ratio and type of polymerization are listed in Table 1. All materials, used in this study, were prepared according to the manufacturers’ instructions. A total of 80 rectangular specimens with a cross-sectional area of 40mm ×10 mm and thickness of 3mm were fabricated from heat-polymerized PMMA as the denture base material for the hardness test. These specimens were prepared by placing two metal plates (stainless steel) upon each other in a conventional denture flask with the aforementioned dimensions. The metal plates were invested in hard but flexible silicone rubber (LasticXtra; Kettenbach, Eschenburg, Germany) to facilitate the removal and the replacement of the plates and the specimens while maintaining the shape. The upper metal plate was removed, denture base resin material was mixed and packed into the mold while the other metal plate was still present in the mold to act as a spacer and maintain 3mm space for the resilient lining material. The flask was placed under pressure in a standard flask press (No.01001; Teledyne Hanau. Buffalo; NY, USA) for 15 minutes; and denture base material was cured in a water bath at 75oC for 9 hours. After polymerization, processed denture base resin plate was removed from the flask and was trimmed. The metal spacer was then removed from the mold, PMMA block was placed back into the mold and temporary soft liner was packed against PMMA into the 3-mm space available on the block and the flask was placed under pressure in the flask press for 15 minutes.
Safari A., et al.
The specimens were removed from the flask and any flash was trimmed with a sharp blade No: 15 (Swann Morton; England) (Figure 1).
J Dent Shiraz Univ Med Sci., Dec. 2013; 14(4): 178-183.
Results There was no significant interaction between soft liners and drinks for both hardness (p= 0.748) and bond strength (p= 0.902) as indicated by the 2-way ANOVA (Tables 2 and 3). Table 2 Two-way ANOVA results for comparison of hardness values
Figure 1a Specimens ready for hardness test b Specimens ready for tensile test
The specimens of both soft liners were divided into 4 groups (n=10) and were immersed in distilled water as the control group, Coca-Cola (Neysun shargh Co; Mashhad, Iran), 8% and 50% ethanol. All groups were stored in separate containers at 37oC, for 12 days. All beverages were exchanged daily. It is reported that 3.2 doses are consumed daily by a regular drinker and each dose lasts for 15 minutes. The 24-hour- storage time simulates one month of regular drinking . Thus, the 12-day-immersion period in this study represents one year consumption of that beverage. The hardness was determined using a Shore A durometer tester (The Shore Instrument & Mfg Co Inc.; Freeport, NY, USA), which was calibrated according to ASTM D2240 and the results were reported in Shore units. For the tensile test, 10 pairs of cylindrical specimens (30mm in height and 10mm in diameter) were prepared for each group by investing two stainless steel dies in front of each other and a 3-mm-thick spacer between them. The PMMA cylinders were fabricated in the flasks as previously described for the hardness specimens. Afterwards, the spacers were removed from the mold and the soft liner materials were mixed, packed into the flasks and were placed under pressure for 15 minutes. The specimens were then removed from the flask and any flash was trimmed with a sharp blade No: 1. Tensile bond strength was determined using Zwick/Roell testing machine (ZwickRoell; Germany) when the failure have occurred and the magnitude of the force was recorded. The bond strength was calculated as maximum load (N) divided by the cross-sectional area (mm2) and reported in mega Pascal (MPa). Two-way ANOVA and Tukey HSD post hoc tests were used to analyze the data. All tests were performed at a preset alpha level of .05 (α=.05) using statistical software (SPSS version 11.0 SPSS Inc.; Chicago, Ill).
Source Soft liner Drink Soft liner x drink Error Total
SS 0.086 4103.871
df 1 3
MS 0.086 1367.957
F P 0.010 0.922 153.346